Isolated π-Interaction Sites in Mesoporous MOF Backbone for Repetitive and Reversible Dynamics in Water.
Xu, Xiaohui; Li, Shenhui; Liu, Qi; Liu, Zhiyu; Yan, Wei; Zhao, Ligong; Zhang, Wenhao; Zhang, Liang; Deng, Feng; Cong, Hengjiang; Deng, Hexiang; ACS applied materials & interfaces 11 (2019) 973–981; doi:10.1021/acsami.8b19211

data_4515434
_publ_section_title
;
 Isolated \p-Interaction Sites in Mesoporous MOF Backbone for Repetitive
 and Reversible Dynamics in Water.
;
_journal_issue                   1
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              973
_journal_page_last               981
_journal_paper_doi               10.1021/acsami.8b19211
_journal_volume                  11
_journal_year                    2019
_chemical_formula_moiety         'C216 Cu3 N12 O32 Zr6'
_chemical_formula_sum            'C216 Cu3 N12 O32 Zr6'
_chemical_formula_weight         4012.22
_space_group_crystal_system      cubic
_space_group_IT_number           221
_space_group_name_Hall           '-P 4 2 3'
_space_group_name_H-M_alt        'P m -3 m'
_atom_sites_solution_primary     dual
_audit_creation_date             2018-08-02
_audit_creation_method
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   25.3953(2)
_cell_length_b                   25.3953(2)
_cell_length_c                   25.3953(2)
_cell_measurement_reflns_used    9991
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      49.797
_cell_measurement_theta_min      2.461
_cell_volume                     16378.0(2)
_computing_cell_refinement       'SAINT v8.34A (Bruker, 2013)'
_computing_data_reduction        'SAINT v8.34A (Bruker, 2013)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'XT (Sheldrick, 2015)'
_diffrn_ambient_temperature      296.15
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.0516
_diffrn_reflns_av_unetI/netI     0.0173
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            40455
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        49.901
_diffrn_reflns_theta_max         49.901
_diffrn_reflns_theta_min         2.460
_exptl_absorpt_coefficient_mu    1.035
_exptl_absorpt_correction_T_max  0.7498
_exptl_absorpt_correction_T_min  0.4970
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2012/1 (Bruker,2012) was used for absorption correction.
wR2(int) was 0.1478 before and 0.0585 after correction.
The Ratio of minimum to maximum transmission is 0.6628.
The \l/2 correction factor is 0.0015.
;
_exptl_crystal_colour            'dark red'
_exptl_crystal_density_diffrn    0.407
_exptl_crystal_description       block
_exptl_crystal_F_000             1963
_refine_diff_density_max         3.303
_refine_diff_density_min         -3.732
_refine_diff_density_rms         0.119
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.116
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     45
_refine_ls_number_reflns         1719
_refine_ls_number_restraints     81
_refine_ls_restrained_S_all      1.308
_refine_ls_R_factor_all          0.1037
_refine_ls_R_factor_gt           0.1009
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1581P)^2^+88.4757P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2706
_refine_ls_wR_factor_ref         0.2737
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1611
_reflns_number_total             1719
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            am8b19211_si_002.cif
_cod_data_source_block           1
_cod_original_cell_volume        16378.0(4)
_cod_database_code               4515434
_shelx_shelxl_version_number     2018/3
_olex2_refinement_description
;
1. Restrained distances
 C7_$1-C7 \\sim C8-C8_$1
 with sigma of 0.02
 C7-C7_$2 \\sim C8_$1-C8_$3
 with sigma of 0.02
2. Restrained planarity
 C2, C5, C3, C4
 with sigma of 0.1
3. Uiso/Uaniso restraints and constraints
Uanis(O1) \\sim Ueq, Uanis(O2) \\sim Ueq: with sigma of 0.02 and sigma for
terminal atoms of 0.2
Uanis(Cu1) \\sim Ueq: with sigma of 0.05 and sigma for terminal atoms of 0.1
Uanis(C10) \\sim Ueq: with sigma of 0.02 and sigma for terminal atoms of 0.2
Uanis(C4) \\sim Ueq: with sigma of 0.02 and sigma for terminal atoms of 0.2
Uanis(C5) \\sim Ueq: with sigma of 0.02 and sigma for terminal atoms of 0.1
Uanis(C6) \\sim Ueq, Uanis(C7) \\sim Ueq, Uanis(C8) \\sim Ueq, Uanis(C9) \\sim
Ueq: with sigma of 0.08 and sigma for terminal atoms of 0.2
Uanis(C10) \\sim Ueq, Uanis(C11) \\sim Ueq, Uanis(C12) \\sim Ueq, Uanis(N1)
\\sim Ueq, Uanis(Cu1) \\sim Ueq: with sigma of 0.01 and sigma for terminal
atoms of 0.1
Uanis(C10) \\sim Ueq, Uanis(C12) \\sim Ueq, Uanis(C11) \\sim Ueq, Uanis(N1)
\\sim Ueq, Uanis(Cu1) \\sim Ueq: with sigma of 0.08 and sigma for terminal
atoms of 0.15
Uanis(C6) \\sim Ueq, Uanis(C7) \\sim Ueq, Uanis(C9) \\sim Ueq, Uanis(C8) \\sim
Ueq: with sigma of 0.05 and sigma for terminal atoms of 0.15
Uanis(C12) = Uanis(C11) = Uanis(C10) = Uanis(N1) = Uanis(Cu1)
Uanis(C2) = Uanis(C3) = Uanis(C4) = Uanis(C5)
Uanis(C6) = Uanis(C7) = Uanis(C8) = Uanis(C9)
4. Others
 Fixed Sof: C7(0.5) C8(0.5)
;
_shelx_res_checksum              74272
_shelx_hkl_checksum              82825
_shelx_fab_checksum              81622
_olex2_submission_special_instructions 'No special instructions were received'